Available online at www.sciencedirect.com

www.elsevier.com/locate/jmbbm

Research Paper

Characterization of uniaxial stiffness of extracellular matrix embedded with magnetic beads via bio-conjugation and under the inﬂuence of an external magnetic ﬁeld Sahan C.B. Heratha,b, Yue Dua,b, Dong-an Wangc, Kin Liaoc, Qingguo Wange, Harry Asadab,d, Peter C.Y. Chena,b,n a

Department of Mechanical Engineering, National University of Singapore, Singapore, Singapore Biosystem and Micromechanics Interdisciplinary Research Group, Singapore-MIT Alliance for Research and Technology Program, Singapore, Singapore c Division of Bioengineering, Nanyang Technological University, Singapore, Singapore d Department of Mechanical Engineering, Massachusetts Institute of Technology, MA, USA e Department of Electrical and Computer Engineering, National University of Singapore, Singapore, Singapore b

art i cle i nfo

ab st rac t

Article history:

In this paper, we study the deformation, and experimentally quantify the change in

Received 14 June 2013

stiffness, of an extracellular matrix (ECM) embedded with magnetic beads that are bio-

Received in revised form

conjugated with the collagen ﬁbers and under the inﬂuence of an external magnetic ﬁeld.

13 November 2013

We develop an analytical model of the viscoelastic behavior of this modiﬁed ECM, and

Accepted 14 November 2013

design and implement a stretch test to quantify (based on statistically meaningful

Available online 28 November 2013

experiment data) the resulting changes in its stiffness induced by the external magnetic ﬁeld. The analytical results are in close agreement with that obtained from the experiments. We discuss the implication of these results that point to the possibility of creating desired stiffness gradients in an ECM in vitro to inﬂuence cell behavior. & 2013 Elsevier Ltd. All rights reserved.

1.

Introduction

The microenvironment surrounding cells plays an important role in inﬂuencing their behavior, e.g., migration, proliferation and differentiation. Two groups of factors exert such inﬂuence: the soluble cues and the insoluble cues. The ﬁrst group concerns biochemical means, including growth factors (such as the vascular endothelial growth factor, VEGF), metabolites and dissolved gases, while the second group involves structural and mechanical properties, such as n

Corresponding author. E-mail address: [email protected] (P.C.Y. Chen).

1751-6161/$ - see front matter & 2013 Elsevier Ltd. All rights reserved. http://dx.doi.org/10.1016/j.jmbbm.2013.11.012

composition, architecture and elasticity of the extracellular matrix (ECM) and cell–cell interactions. Developing comprehensive knowledge about cell behavior in culture remains a challenge in basic biological research (Hansen and Bissell, 2000), drug discovery (McNeish, 2004), tissue engineering, and regenerative medicine (Guillot et al., 2007). Incorporating all these cues in the microenvironment for in vitro cultivation of cells is a crucial step in gaining such knowledge. Signiﬁcant advances have been made on ﬁnding the appropriate mixture of soluble cues in liquid media for

254

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

culturing various types of cells, while the effect of insoluble cues remains a fertile area to be explored (Ludwig et al., 2006; Lu et al., 2006; Soen et al., 2006; Nakajima et al., 2007). It is interesting to note that the impact of insoluble cues in fact could be far more important than previously thought, as is illustrated in the case of mammalian cell and human mesenchymal stem cell differentiation (Keung et al., 2010). The stiffness of the ECM (an insoluble cue) is known to inﬂuence many types of cellular behavior (Pelham and Wang, 1997; Assoian and Klein, 2008). Cells within tissues can sense the mechanical stiffness of both the ECM and other cells. ECM stiffness regulates the degree of cell-matrix adhesion, the size of the focal adhesion, as well as the stiffness and tension developed by the cell itself (Wells, 2008; Engler et al., 2006). Motility and cell alignment are also associated with ECM stiffness, manifested in the tendency of cells to migrate from softer to stiffer environment (Harland et al., 2011). At the basic level, ECM stiffness can regulate cell growth and viability, as well as resistance to apoptosis. Although the mechanisms of many of these effects are still unknown, it is generally accepted that the mechanical properties of the ECM inﬂuence cell biology at various levels, including protein expression (Zaman et al., 2006). A number of methods have been proposed in the literature for changing the stiffness of collagen for the purpose of observing in vitro cell behavior in an ECM sample (Alfredo Uquillas et al., 2012; Kane and Roeder, 2012). One involves changing collagen concentration, as demonstrated in the work by Helary et al. (2010). Another method involves varying the pH value in a sample, since solution acidity during ﬁbrillogenesis affects collagen stiffness. Silver et al. showed that the Young's modulus of an ECM sample changed from 0.5 MPa to 5.5 MPa when the pH value was reduced from 8.5 to 6 at 37 1C (Christiansen et al., 2000). Changing the temperature of an ECM sample can also lead to change in its stiffness. The Young's modulus of ECM samples has also been shown to increase with polymerization temperature, e. g., from 0.3 Pa at 4 1C to 22.7 Pa at 37 1C (Raub et al., 2007). These currently known methods mainly rely on manipulating soluble cues. Manipulating the stiffness of ECM by mechanical means offers an alternative to approaches that rely on soluble cues. Recent results have demonstrated the possibility of changing mechanical and rheological properties of composites with highly elastic polymer matrices that are ﬁlled with magnetic particles (Stepanov et al., 2007; Wang et al., 2006). It had been reported that these materials show signiﬁcant change in their mechanical properties under the inﬂuence of magnetic ﬁelds. We have recently proposed an approach to alter the stiffness of ECM samples by mechanically manipulating the deformability of the collagen ﬁbers in the ECM. A very brief description of the concept underlying this approach was initially presented (with limited preliminary experimental data) in (Chen et al., Asada). This approach involves embedding micron-size magnetic beads in an ECM sample (hereafter referred to as a modiﬁed ECM sample) through bioconjugation between the streptavidin-coated beads and the collagen ﬁbers, then applying an external a magnetic ﬁeld on the sample to exert a magnetic force on the beads. Embedding a single or very few superparamagnetic particles in the

ECM in order to probe cells or to manipulate cell-ECM interaction is a well-known practice (Chippada et al., 2009; Alenghat et al., 2000; Bausch et al., 1998). The novelty of our proposed approach manifests in the ability to directly manipulate an ensemble of such magnetic particles to alter the apparent stiffness of the macrostructure. While the basic concept and some very preliminary results have been brieﬂy reported in Chen et al. (Asada), to develop this approach into a practical technique for in vitro manipulation of cellular behavior requires a substantive quantitative characterization of the effect of an external magnetic ﬁeld on the stiffness of the modiﬁed ECM. The work reported in this paper focuses on establishing such a characterization by means of both detailed analytical modelling and extensive experimental investigation. Speciﬁcally, in this paper we investigate the effect of an external magnetic ﬁeld on the uniaxial stiffness of modiﬁed ECM samples by (i) developing an analytical model (described by a set of constitutive equations) of the behavior of the modiﬁed ECM under the inﬂuence of an external magnetic ﬁeld, (ii) designing and implementing a stretch test to quantify such changes based on statistically meaningful data collected from a set of carefully designed experiments, and (iii) evaluating the effectiveness of this approach by comparing the analytical and the experimental results. The remainder of this paper is organized as follows. Section 2 presents an overview of the approach and the general principles in the design of the experiments. Section 3 develops an analytical model describing the viscoelastic behavior of the modiﬁed ECM samples under the inﬂuence of an external magnetic ﬁeld. Section 4 describes the design and the implementation of the experiments and presents the results. Section 5 evaluates the results from the analysis and the experiments, and discusses the implication of the results and directions for further research to improve the practicality of the proposed approach.

2.

Approach

Superparamagnetic beads are embedded in the ECM via bioconjugation between the beads and the ECM ﬁbers. The beads are coated with streptavidin that enables the formation of strong covalent bonds between the beads and the collagen ﬁbers in the ECM, as is illustrated in Fig. 1a. Applying an external magnetic ﬁeld on the beads produces a pre-tension (along in the direction of the magnetic ﬁeld) in a region in the ECM due to the magnetic forces experienced by the beads. This externally created pre-tension can be conﬁgured to generate resistance to the deformation of the collagen ﬁbers in that region, which in turn affects the deformation of the ECM. This resistance to deformation manifests in the change in the apparent stiffness of the ECM. We characterize this change in the apparent stiffness in one dimension in the setting of a stretching test, as is illustrated in Fig. 1c. A modiﬁed ECM strip is ﬁxed at one end while the other end is stretched. During the stretching, two magnets (one on each side of the ECM strip) produce two magnetic forces on the individual beads. Each of these two forces can be resolved into two components: one along the

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

255

Fig. 1 – Illustration of the proposed approach.

axis of stretching and point towards the center line between the two magnets, while the other pointing towards a magnet. Fig. 1c illustrates this situation for the case where the bead is initially located near the center line of the two magnets. The distribution of deformation in the collagen can be observed from Fig. 1b, which shows a greater deformation in the region of the ECM closer to the free moving end than in the ﬁxed end. Since the deformation is greater at the point where the stretching force is applied and reduces linearly to zero at the ﬁxed end, the beads located above the magnets are displaced more signiﬁcantly than the beads located below the magnets. The beads above the magnet experiences a downwards force that opposes the deformation of the collagen. Therefore a larger force is required to overcome these forces while stretching. The magnetic ﬁeld also induces forces on the beads perpendicular to the direction of stretching. This force will also reduce the tensile deformation caused by the stretching force.

3.

Modelling of ECM deformation

In a modiﬁed ECM sample, the beads (with a diameter of approximately 1.5 μm) are thoroughly mixed with the collagen solution to ensure a uniform distribution. At a typical bead concentration of $0.1$ to $0.5$ mg/ml, the number of beads is in the order of 108. Such a large number of beads pose a problem in constructing a model for describing the viscoelastic behaviour of the modiﬁed ECM using existing FEM techniques, since in these techniques the beads need to be accounted for individually. A model is thus developed to analyze the structural mechanics of the modiﬁed ECM in which the ECM is treated as viscoelastic and subjected to numerous distributed point loads generated by the magnetic beads when under the inﬂuence of a magnetic ﬁeld.

3.1.

Model of ECM deformation under internal point loads

The viscoelasticity of the ECM (prepared from Rat Tail Collagen Type I) is modelled by using the Standard Linear Solid Model (SLSM), which consists of two springs and a damper, as is illustrated in Fig. 2. Compared to the Maxwell model and the Kelvin–Voigt model, the SLSM describes the deformation behaviour of viscoelastic material more

Fig. 2 – The Standard Linear Solid Model (SLSM) consists of two springs (represented by the spring constants E1 and E2, and a dash-pot with a damping coefﬁcient η.

accurately. An instantaneous elastic deformation is observed when a viscoelastic material experiences an instantaneous stress. The existence of E2 in the SLSM contributes to the improved accuracy in the model for describing such an instantaneous deformation (Elias and Spector, 2012). From this conceptual model shown in Fig. 2, various constitutive equations that link stress with strain have been developed (Kaliske and Rothert, 1997; Savage et al., 2010; Saffar and Abdullah, 2013; Lim et al., 2006). The method employed in the derivation of viscoelastic deformation (due to an external force) of an ECM sample follows the principle of minimum potential energy. This method seeks to determine a deformation state of the ECM corresponding to a minimum potential energy over all possible deformation states (Chandrupatla et al., 1991) (The notations of some parameters in (Chandrupatla et al., 1991) are used in this paper). The potential energy πp is deﬁned as π p ¼ π s Wp ; T ε and the where πs is the strain energy involving the strain ! ! stress s , and is given by Z Z Z 1 T ! ε ! s dV πs ¼ 2 V

while Wp is the work done on the ECM by the external force, i. e., Z Z Z Z Z !T ! !T ! !T ! Q f dV þ Q Φ dS þ ∑ Q i P i Wp ¼ V

S

i

! ! ! ! with Q being the displacement vector, f , Φ and P i the body force vector, the surface force vector, and the point force vector, respectively, V the volume of the ECM, and S the surface of the ECM that experiences the surface force.

256

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

The stress ! s is derived based on the viscoelastic constitutive model developed in Kaliske and Rothert (1997). The total stress ! s is given as ! s2 s ¼! s1þ! with ! s 1 and ! s 2 being the elastic stress generated in the ! ε ¼ BQ (with B spring E1 and spring E2, respectively. From ! being the derivative of the shape function with respect to the ! physical coordinates), we can express ! s 1 as D1 BQ , where D1 represents the relationship between the stress and the strain s 2 for the in three dimensions for the spring E1. The stress ! spring E2 can be estimated recursively as Δt=τ

1 e Δt nþ1 n ! e τ ! s 2 þα s2 Δt=τ

ð! s1

nþ1

! s1 Þ n

where τ ¼ E2 =Z is the time constant, and α is the relative s is stiffness E2/E1. Hence, the total stress ! Δt=τ

1 e Δt nþ1 nþ1 n ! ! s1 þ e τ ! s2 þα s Δt=τ

nþ1 ! n ð! s1 s1 Þ

ð1Þ

The numerical approach based on the ﬁnite element method is applied for analyzing the structural mechanics of the modiﬁed ECM. The ECM is meshed into a total of m fournode linear tetrahedron elements. The generated nodal

displacements can be converted to the displacement at any point in the ECM. The potential energy at time step (nþ1) is ZZZ 1 !nþ1T m nþ1 BT ! ∑ s dV π pnþ1 ¼ Q 2 e¼1 Ve 0 1 ZZZ ZZ nþ1 !nþ1 !nþ1T m @ T T! Q N f ∑ dV þ N Φ dSA e¼1

!nþ1T !

Q

S

P i:

ð2Þ

The deformation state corresponding to a minimum !nþ1 ¼ 0 leadpotential energy is obtained by solving ∂π nþ1 p =∂ Q ing to the formula to generate the nodal displacements at time step (nþ1), i.e., !n αð1 e nΔt=τ Þ !nþ1 1 nþ1 1 ¼ ðKinst Þ Kc Q Q 2 nΔt=τ ! 0 T !n nΔt ðB Þ s e τ þ F ð3Þ 2

nodes

where, Kc is the assembly of element stiffness matrix Kce ¼ V e BTe DBe for the spring E1, with D (which is the same as D1) describing the relationship between the stress and the strain in three dimensions relevant to E1 and the Poisson's ratio, B0 is the assembly of BTe Ve, with Be and Ve being the matrix of the derivative of the shape function and the volume nþ1 is the assembly of the of the element, respectively, Kinst instantaneous element stiffness matrix, i.e., αð1 e nΔt=τ Þ Kc ¼ 1 þ Knþ1 inst nΔt=τ ! and F nodes is the nodal force, i.e., 0 1 ZZ ZZZ m nþ1 !nþ1 ! ! ! T T F nodes ¼ ∑ @ dV þ N Φ dS þ P i A N f e¼1

Fig. 3 – Model of the ECM sample with point loads due to the virtual beads.

Ve

Ve

S

Since the streptavidin-coated beads are bound to the collagen ﬁbers and experience magnetic forces, their impact ! on the ECM can be considered as point forces P i , as is illustrated in Fig. 3, where the arrangement of the beads ! and magnetic forces P mimics the conditions in the stretchtest experiment. In the experiment, the ECM is subjected to two groups of point forces pointing outwards (and perpendicular to its length) in opposite directions. Fig. 4a shows the

Fig. 4 – (a) von Mises stress generated in the ECM, and (b) the z-directional deformation of the top surface (S1) of the ECM.

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

257

von Mises stress while Fig. 4b shows the deformation of the ECM sample in the z direction. From these ﬁgures, it can be observed that larger stress is generated around the beads. The combined inﬂuence of the beads results in the contraction of the ECM in the negative z-direction.

3.2. Determination of apparent stiffness of modiﬁed ECM under the inﬂuence of an external magnetic ﬁeld Let Epure, Ebead, and Emod denote the Young's modulus of the pure ECM, the modiﬁed ECM in the absence of the magnetic ﬁeld, and the modiﬁed ECM in the presence of the magnetic ﬁeld, respectively. We now apply the analytical model developed in Section 3.1 to determine Emod based on Epure, Ebead, and the magnetic force acting on the beads due to the magnetic ﬁeld. This magnetic force is generated by a pair of magnets (described later in Section 4.3, and its magnitude is computed based on the approach presented in (Lipfert et al., 2009). In the analytical model, the effect of the external magnetic ﬁeld on the ECM is accounted for in terms of the point forces generated by the (virtual) beads in the ECM. In this context, the stiffness of a modiﬁed ECM sample under the inﬂuence of an external magnetic ﬁeld can be expressed as the sum of the following two terms: (i) the apparent stiffness of the pure ECM subjected to the pretension induced by the point forces representing the magnetic forces acting on the beads (denoted by Epoint, and (ii) the increase in the Young's modulus of the ECM solely (i.e., without the magnetic ﬁeld) due to the presence of the magnetic beads (denoted by ΔEbead); that is, ΔEbead ¼ Ebead Epure.

We thus write, Emod ¼ Epoint þ ΔEbead

ð4Þ

The term Epoint (due to the pre-tension in the pure ECM) can be determined as follows. We ﬁrst calculate the pretension using Eq. (3), based on the magnetic forces exerted in the ECM through the beads and the stiffness of the pure ECM. Speciﬁcally, Kc and Knþ1 inst in Eq. (3) are obtained, using Eq. (4), from the stiffness of the pure ECM, which is determined by ! experiment as described later in Section 5.1, while F nodes takes on the values of the magnetic forces. In this case, the beads are considered “virtual” in the sense that the modiﬁed ECM is constitutively the same as the pure ECM—other than the existence of the “virtual” point loads when the magnetic ﬁeld is present. The portion of force required to overcome this pre-tension is then calculated and added to the force that is needed to deform the pure ECM for a given deformation, leading to the total force required to produce that deformation in the modiﬁed ECM in the presence of a magnetic ﬁeld. Fig. 5 shows the total forces required to deform the ECM at a constant rate of 10 mm/min in the presence of the magnetic ﬁeld for different concentrations of beads. For the pure ECM, this force increases linearly under a constant rate of elongation. By contrast, for the ECM with beads exposed to the magnetic ﬁeld, this force increases exponentially under the same rate of elongation. It can be also seen that a greater

Fig. 5 – Force-deformation relationships for three types of ECM, i.e., pure ECM, ECM with beads at a concentration of 0.1 mg/ml and 0.5 mg/ml. The ECM with beads is exposed to an external magnetic ﬁeld created by a pair of permanent magnets.

Table 1 – Apparent stiffness of modiﬁed ECM exposed to an external magnetic ﬁeld, obtained from numerical simulation. Bead concentration (mg/ml)

Apparent stiffness (N/mm)

0.1 0.5

0.0053 0.0103

force is required to deform the ECM with beads exposed to the magnetic ﬁeld as compared to the case of pure ECM. Moreover, the increase in bead concentration is associated with the growth of the force. The reason is that the increase in bead concentration causes a larger pre-tension that resists ECM deformation. Now the term Epoint in Eq. (4) can be calculated by linearizing the force-deformation curves after the transition point as shown in Fig. 5. The region before this transition point is the creep region commonly found in viscoelastic deformation. The slope of the curve after the transition point is used to determine Epoint (Pedro Kato et al., 1989; Fratzl et al., 1998). To obtain Emod, ΔEbead is then calculated based on ΔEbead and Epure, which are obtained from the experiments (discussed in Section 5). Table 1 shows the values of Emod thus obtained for two types of ECM samples with different bead concentrations. It can be seen that increasing the concentration of beads from 0.1 mg/ml to 0.5 mg/ml leads to a signiﬁcant increase in the apparent stiffness of the modiﬁed ECM. Comparison between results from numerical simulation (using the analytical model) and that obtained experimentally is presented in Section 5.5.

4.

Experiment

We embedded magnetic beads in the ECM and evaluated its apparent stiffness empirically. The stiffness evaluation involved three types of ECM samples: (i) pure ECM without any beads, (ii) ECM embedded with beads that were bio-conjugated with the

258

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

Table 2 – Recipes for collagen preparation. Components

Without magnetic beads (ml)

With magnetic beads (0.1 mg/ml) (Streptavidin coated) (ml)

With magnetic prbeads (0.5 mg/ml) (Streptavidin coated) (ml)

With magnetic beads (0.5 mg/ml) (PEG-coated) (ml)

Collagen (4.62 mg/ml) Water PBS (10 ) NAOH (0.5 N) Beads (5 mg/ ml)

1.593

1.593

1.593

1.593

1.089 0.325 0.244 0

1.024 0.325 0.244 0.065

0.764 0.325 0.244 0.325

0.764 0.325 0.244 0.325

3.250

3.250

3.250

3.250

Total

collagen ﬁbers, and (iii) ECM embedded with beads that were not bound to the collagen ﬁbers.

4.1.

Embedding beads in ECM

To embed beads in the ECM with bio-bioconjugation, magnetic beads were prepared with a coating having a good afﬁnity with the collagen ﬁbers to form a strong attachment. We used beads coated with streptavidin since streptavidin will afﬁx to areas dense with collagen. Streptavidin contains an Arg-Tyr-Asp (RYD) amino acid sequence that mimics the Arg-Gly-Asp (RGD) receptor domain of ﬁbronectin (Guo and Kaufman, 2007). This form of bio-conjugation involves four types of bonding, namely, hydrophobic, van der Waals, hydrogen bonding network, and covalent bonds. The complementary shapes, charges, polarity, and hydrophobicity of the streptavidin and the collagen ﬁbers permit multiple weak interactions which in combination produce a tight binding (Stenkamp et al., 1997; Lodish, 2008). To embed beads in the ECM such that there is no binding between the beads and the collagen ﬁbers, Polyethylene glycol (PEG) coated beads were used. Due to its hydrophilicity, this coating prevents bio-conjugation from occurring between the collagen ﬁbres and the beads. PEG coating is done on the amine coated beads so that it creates an inert coating around the beads. The PEG structure contains hydrogen bonded to water molecules that results in a hydration layer, which makes bonds between the PEG coated beads and the collagen ﬁbres difﬁcult to form since this layer must be disrupted for any form of bio-conjugation to occur. The detailed procedure is described in Appendix A.

Fig. 6 – Teﬂon mold for collagen formation.

groups of samples were prepared: one with magnetic beads and one without. For samples with magnetic beads, two different concentrations, i.e., 0.1 mg/ml and 0.5 mg/ml, of the beads were added (as indicated in Table 2). A PTFE mold with a through hole and a base was fabricated and used to contain the liquid collagen until gellation occurred. The dimensions of this mold are shown in Fig. 6. The collagen (or the collagen with beads mixture) was thoroughly vortexed for two minutes until a homogeneous solution was formed and all the components of the mixture were spread throughout the entire volume. The mixture was then pipetted into the mold carefully so that no visible air cavities were formed. Fibrillogenesis was usually done in an external incubator at 37 1C and 5% CO2. To achieve selfassembly of collagen molecules into ﬁbers and binding of beads to the collagen ﬁbers, the samples were placed in an incubator for at least 22 h to ensure that gellation occurred throughout the entire collagen strip.

4.3. 4.2.

Experiment setup and procedure

Preparation of samples

The collagen was prepared according to the recipes listed in Table 2. All of the samples contain 2.0 mg/ml of Rat Tail Collagen Type 1, obtained from BD Biosciences. The streptavidin-coated magnetic beads, BM551, were procured from Bangs Laboratory. To enable conjugation of Polyethylene glycol (PEG) to the magnetic beads requires beads with an amine functional end group. The amine-coated magnetic beads, BM546, were procured from Bangs Laboratory and the PEG (at 3400 g/mol) was procured from Sigma Aldrich. Two

The stiffness of the ECM was evaluated by a stretch test using an Instron 8848 micro-force tester. The micro-force tester has a load cell rated at 10 N with a 0.001 N resolution. Stretch tests were carried out on ECM samples at the ﬁxed rate of 10 mm/min. While performing the stretch tests, a certain portion of the sample was exposed to a static magnetic ﬁeld produced by a permanent magnet, as is depicted in Fig. 7. This permanent magnet is made of an alloy of neodymium, iron and boron (NdFeB) and it is capable of producing a magnetic ﬁeld of 0.2 T. Two magnets form an

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

4.4.

259

Data processing

The full stretch graph from one sample is shown in Fig. 8a and b shows the linear section of the curve that is used to determine the stiffness of the pure collagen sample. There is a clear distinction of the two set of curves in the elastic region before sample rupture occurs as shown in Fig. 8. It can be observed from Fig. 8b that the sample under the inﬂuence of the magnetic ﬁeld exhibits a steeper slope than the sample without a magnetic ﬁeld. The graphs of each of the stretch tests were plotted and the gradient of the linear section of each graph was extracted. The mean was obtained from the four samples in each set, as shown in Fig. 10.

5.

Results and discussion

5.1.

Determination of pure ECM stiffness

Fig. 7 – Experiment Setup.

Table 3 – Test scenarios. Each set involves four ECM samples. Set no.

Bead concentration

Magnetic ﬁeld

1 2 3 4 5 6 7 8

0 0 0.1 mg/ml 0.1 mg/ml 0.5 mg/ml 0.5 mg/ml 0.5 mg/ml PEG coated 0.5 mg/ml PEG coated

Off On Off On Off On Off On

aligned conﬁguration such that the ECM sample is located between the magnets with a gap of 1.5 cm from each magnet. This leads to the creation of restoring forces on the beads when they are dislocated from their original positions (when the ECM sample is in its un-stretched state) by the stretching action. The introduction of the magnetic ﬁeld thus creates a region of higher stiffness in the ECM such that a larger force is required to produce a given deformation (i.e., elongation, in this case) compared to the amount of force required to produce the same deformation in the absence of the magnetic ﬁeld. The stretch tests were carried out until the ECM ruptures. The force applied on, and the extension of, the ECM were recorded during the test. Eight sets of tests (involving four ECM samples in each set) were conducted under the conditions summarized in Table 3. The ﬁrst two sets involve ECM samples without any beads embedded (i.e., pure ECM samples). These two sets of tests were designed to demonstrate that the magnetic ﬁeld alone does not affect the stiffness of a pure ECM, and to establish a basis on the stiffness of the pure ECM for comparison with the results from the other four sets of tests. The next four sets (i.e., Sets 3–6) investigate the effect of the external magnetic ﬁeld on the stiffness of the modiﬁed ECM. Finally, Sets 7 and 8 examine the effect of the presence of the beads (in the ECM but without any bio-conjugation between the beads and the collagen ﬁbers) on the ECM stiffness.

The stiffness of pure ECM is obtained from linear-ﬁtting of the force-deformation curve of pure ECM generated from experimental data. The parameter E1 in the SLSM model (shown in Fig. 2) determines the steady-state deformation of the ECM under external forces, while E2 is only relevant to the rate of approaching the steady deformation. Here E2 is randomly chosen to be $500$ Pa in the simulation as it has negligible impact on the result concerning the change in ECM stiffness. The parameters E1 and η were obtained by linearﬁtting of the force-deformation curves shown in Fig. 9, which were obtained experimentally. The thick straight line in the ﬁgure is the result of the linear-ﬁtting, whose slope is the stiffness of the pure ECM, while the initial offset is related to the viscosity of the pure ECM. Based on this stiffness, the Young's modulus of the pure ECM Epure E1 is calculated from Epure ¼ k L/A, with the stiffness k¼ 0.003 N/mm, the cross-sectional area of the ECM A¼ 48 mm2, and the length of the ECM L ¼28 mm. (In the experiment the original length of the ECM samples was 33 mm. With the two ends of the sample clamped by the micro-force tester, the effective length of the ECM was thus reduced by 5 mm.) The Young's modulus Epure is calculated to be 1750 Pa. The offset z in Fig. 9 is used to calculate the viscosity η of the ECM based on the equation η ¼ z L/(A_ε), with z¼0.0023 N and the deforming rate ε_ ¼ 10 mm/min (which is the rate used in the experiment). The viscosity of the ECM is calculated to be 134 Pa min.

5.2. Change in stiffness of modiﬁed ECM induced by the external magnetic ﬁeld Fig. 10 shows the results of the eight sets of tests done on a total of 32 ECM samples. Cross-test comparison provides direct quantiﬁcation of the effect of (i) the bio-conjugated beads, (ii) the bio-conjugation, and (iii) the external magnetic ﬁeld, on the uniaxial stiffness of the ECM samples, as summarized in Table 4. Comparison of results from Set 1 and Set 2 reveals that the pure ECM samples exhibit similar stiffness, regardless of whether the magnetic ﬁeld was on or off. As is shown in Table 4, the average stiffness of pure collagen with and without the magnetic ﬁeld differs by 5 10 4 in magnitude.

260

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

Fig. 8 – (a) Stretch test result of a sample embedded with beads at a concentration of 0.5 mg/ml and in the presence (solid curve) and absence (dotted curve) of a magnetic ﬁeld. (b) Linear sections of the graphs taken to estimate the stiffness of two samples.

Fig. 9 – Force-deformation relationship of pure ECM samples.

261

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

Fig. 10 – Summary of results from experiments. Table 4 – Summary of two-tailed P values from unpaired t tests and difference in magnitude of the mean values of stiffness. The numbers in brackets have the same meanings as those labeled on the bars in Fig. 10; the top number in each entry indicates the P value while the bottom number indicates the difference in the mean value of stiffness. (1) (2) (3)

(5)

(7)

0.5718 5 10 4 0.8084 2 10 4

(4) (5)

(3)

0.0085 2.2 10 3 0.0234 3.3 10 3

(6)

0.0605 4.3 10 3

(8)

The unpaired t-test shows that the two-tailed P value equals 0.5718; this difference is considered to be not statistically signiﬁcant. It can therefore be concluded that the magnetic ﬁeld had no signiﬁcant effect on the stiffness of the pure ECM samples, and that the differences among the force–displacement relationships of the eight samples (in this set) were due to sample variations attributed to the repeatability of the ECM preparation process. The average slope of the linear approximation of the force–displacement relationship (calculated from data of Set 1 and Set 2) is 3 10 3 N/mm. The effect of the mere presence of bio-conjugated beads in a ECM sample can be studied by comparing the results of Set 1 and Set 3. It can be seen, from both Fig. 10 and Table 4, that embedding beads in a pure ECM sample (in the absence of an external magnetic ﬁeld) slightly increases its uniaxial stiffness. To examine how an external magnetic ﬁeld may affect the uniaxial stiffness of modiﬁed ECM samples, we compare the results from Set 5 and Set 6. It can be observed that there is a signiﬁcant increase in the stiffness when the magnetic ﬁeld is in

0.7259 4 10 4

effect. Similar conclusion can be drawn for the case involving Set 3 and Set 4, where the beads are at a lower concentration. We next investigate the case where the embedded beads are not bound to the ECM ﬁbers. To see the effect (if any) of such no-binding beads on the stiffness of the ECM, stretch test results are obtained from experiments Set 7 and Set 8. From Fig. 10 and Table 4, it can be seen that the stiffness of the ECM samples embedded with non-binding beads (i.e., beads coated with PEG) is signiﬁcantly lower than that of the samples with beads coated with streptavidin (and thus bioconjugated to the ECM ﬁbers). This is expected since the beads not bound to the ECM ﬁbers offer, when under the inﬂuence of the external magnetic ﬁeld, much weaker resistance against the dislocation of the ﬁbers during ECM deformation.

5.3. Stiffness of ECM with streptavidin-coated magnetic beads Fig. 10 and Table 4 indicate that the external magnetic ﬁeld produced signiﬁcant changes in the stiffness of the modiﬁed

262

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

ECM. Speciﬁcally, the increase is 63% in the case of Set 6 (i.e., from 0.0068 N/mm to 0.0111 N/mm). A similar observation can be made for Set 4, which shows an increase in stiffness of 59% (i.e., from 0.0037 N/mm to 0.0059 N/mm). Furthermore the stiffness of the modiﬁed ECM with a lower concentration of beads is very close to that of the pure collagen when the magnetic ﬁeld is off (i.e., Set 3 and Set 1). This clearly indicates that embedding beads at a low concentration alone will not signiﬁcantly alter the mechanical properties of the modiﬁed ECM; the change in stiffness becomes signiﬁcant only when an external magnetic ﬁeld is applied.

5.4.

Stiffness of ECM with PEG coated magnetic beads

For Set 7 and Set 8, the change in stiffness of 7% (i.e., from 0.0056 N/mm to 0.0060 N/mm) is not as signiﬁcant compared to an increase of 63% for the case of Set 5 and Set 6. This indicates that the binding between the beads and collagen ﬁbers indeed plays a signiﬁcant role in altering the overall stiffness of the ECM when a magnetic ﬁeld is applied. Such binding enables the collagen ﬁbrils to attach to the beads strongly, resulting in a greater resistance to deformation in the ﬁbers when an external magnetic ﬁeld generates magnetic forces that oppose the movement of the beads.

5.5. Comparison of ECM apparent stiffness obtained from simulation and experiment Table 5 shows the values of the Young's modulus of the modiﬁed ECM obtained from the model presented in Section 3 and from the experiments. It can be seen that the analytical results are in close agreement with that obtained from the experiments.

Table 5 – Comparison of Young's modulus of modiﬁed ECM. Bead concentration (mg/ml)

Simulation

Experimental (Streptavidin-coated)

0.1 0.5

0.0053 0.0103

0.0059 0.0111

6.

Concluding remarks

We have demonstrated, by analytical modelling and experiment, that the uniaxial stiffness of the ECM can be altered actively to a signiﬁcant degree by embedding (in the ECM) magnetic beads that are bio-conjugated with the collagen ﬁbers and applying an external magnetic ﬁeld. The experimental results point to the possibility of creating desired stiffness gradients in an in vitro extracellular matrix to inﬂuence various cell behavior, such as proliferation, differentiation and apoptosis. The exertion of such inﬂuence can be interpreted in the context of the forcebearing interaction between cells and the collagen ﬁbers.

6.1.

Utility of the proposed ECM deformation model

In Section 3, we propose a new model for describing the viscoelastic behavior of the modiﬁed ECM. Speciﬁcally, we show that the Young's modulus of the modiﬁed ECM under the inﬂuence of an external magnetic ﬁeld can be determined analytically based on Epure, Ebead, and the magnetic force acting on the beads due to the magnetic ﬁeld. The advantage of having this model is that it enables the determination of the stiffness of a modiﬁed ECM sample corresponding to a given external magnetic ﬁeld without having to conduct a stretch test on the sample involving the instrumentation for the generation of that speciﬁc external magnetic ﬁeld. This is particularly useful in an application where the stiffness of the modiﬁed ECM is being actively manipulated by dynamically varying the strength of the external magnetic ﬁeld. In such a case, the model offers an efﬁcient way to determine the instantaneous value of the Young's modulus of the modiﬁed ECM.

6.2. Implication of the proposed method for active manipulation of ECM stiffness Application of an external magnetic ﬁeld on a modiﬁed ECM sample creates a pre-tension in the collagen ﬁbers. When a traction force acting in the direction opposite to the magnetic force is exerted on the ﬁbers by a cell, the ﬁbers exhibit a greater resistance to deformation, as is illustrated in Fig. 11. Due to this increased resistance to deformation in the ﬁbers, cells will experience a greater stiffness in regions of the ECM where beads are present, which in turn may affect the

Fig. 11 – Schematic illustration of bead-embedded ECM and interaction between collagen ﬁbers and cells via focus adhesion under the inﬂuence of an external magnetic ﬁeld.

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

cell behavior, such as cell migration. We refer to this stiffness sensed by the cells as the apparent local stiffness of the ECM at those sites, since this externally and mechanically induced change in the local deformability of the collagen ﬁbers is only apparent to a cell near the site of an embedded bead and is localized at that site, while the global intrinsic material properties of the ECM remain unchanged. The advantage of this approach is that the stiffness of the ECM can be manipulated directly in real-time without signiﬁcantly changing the in vitro environmental conditions (such as temperature or pH value) for a cell. A number of attempts have been reported in an effort to make practical this approach for active manipulation of ECM stiffness. A pure computational and simulation-based study on the stiffness of the modiﬁed ECM was reported in (Du et al., 2012); it uses a conceptual model constructed by calculating the total stress directly from the strain, which is less efﬁcient than the method used in this paper. Another work focuses on the microscopic stiffness of the ECM in the vicinity of a magnetic bead (Herath et al., 2012). Although there is generally a similarity between micro-scale and macro-scale stiffness for stiffer materials, such a similarity does not apply to soft biological materials. The stiffness of soft materials varies signiﬁcantly when measured in micro- and macro-scale, due to their heterogeneous structures. (We note that the work presented in this paper concerns only macro-scale measurements.) Lastly, the effect of the induced change in stiffness of the modiﬁed ECM on the behaviour of angiogenic sprouting was reported in (Chen et al., 2012). While all these works mentioned above yielded useful insight on the mechanical behavior of the modiﬁed ECM and how that behavior may inﬂuence certain biological behavior of endothelial cells, they remain preliminary and various issues remain to be investigated. First, the effect of a number of variables on the stiffness of the modiﬁed ECM remains to be explored; these variables include bead concentration, size and placement of the magnets and their distance to the ECM sample, and strength of the magnetic ﬁeld, etc. Second, the experiments described in this paper only concern manipulation of ECM stiffness along a single axis. To study how ECM stiffness affects cell behavior in vitro requires the ability to manipulate the stiffness gradient in 3D. Third, although magnetic beads have been used in many applications (both in vivo and in vitro), their effect on the actual biological behaviour of cells are not yet fully understood. This is particularly true when an ensemble of beads are embedded in the ECM via bio-conjugation. It may be argued (based on available experimental results, e.g., (Yanada et al., 2006; Conrad-Lapostolle et al., 1996; Hafeli, 2006)) that the biocompatibility and toxicity of these magnetic beads with respect to its biological environment solely depends on the surface coating that is adhered to the magnetic particle, it is essential to verify that such an ensemble of beads do not directly interfere with the natural behaviour of cells.

263

Singapore-MIT Alliance for Research and Technology Program) for their ﬁnancial support. The ﬁrst author would like to acknowledge the ﬁnancial support provided by the National University of Singapore. The second author also would like to acknowledge the ﬁnancial support provided by the China Scholarship Council and the National University of Singapore.

Appendix A. Preparation of PEG coated magnetic beads The coating on anime functionalised magnetic beads was applied via the following steps (Wang et al., 2003; Soﬁa et al., 1998; Nilsson and Mosbach, 1981). 1. Activation of PEG—Dehydration of PEG was done by dissolving 6.03 g of PEG in 150 ml toluene in a 3 neck ﬂask from which 50 ml toluene/water micellar mixture was extracted by azeotropic distillation. The dehydrated PEG was then mixed with a catalyst, Triethylamine (TEA), in a 3 neck ﬂask which was placed in salt-ice bath. 0.2 ml of Tresylchloride in 50 ml of anhydrous CH2Cl2 was poured into an equalised addition funnel and added dropwise into the 3 neck ﬂask containing the PEG and TEA mixture. The reaction was carried out in an argon atmosphere. It was left for 1 h in ice bath and for another 2 h in room temperature. Magnetic stirring was maintained at 600 rpm throughout the reaction. After which the product was precipitated with 10-folds excess of ethyl ether. The powders were vacuum dried at room temperature in the dark. 2. Coupling of PEG with magnetic beads—The amine coated beads were washed with PBS thrice. Then 0.804 g of PEG was dissolved in 7.5 ml of 10 mM PBS (PH 7.4) and 0.5 ml of magnetic beads suspension. The ﬁnal volume of the mixture was 9 ml. This reaction was carried out in an ice bath for 12 h and for another 12 h in room temperature. Magnetic stirring at 600 rpm was maintained throughout the reaction. 3. Zeta potential test—The zeta potential measurement was carried out to ensure that coupling had occurred between the magnetic beads and PEG. Due to the charge shield effect of PEG, the results of the zeta potential test should show a lower value for the coupled beads compared to the amine coated beads. The beads were washed to change the solution from PBS to Deionised water prior to conducting the tests. The test results (as shown in Table 6) indicates a lower potential in the coupled PEG-bead solution compared to that in the solution of amine bead only. This indicates that PEG coupling had occurred for the amine coated beads.

Table 6 – Zeta potential measurement.

Acknowledgments The authors would like to thank the BioSystem and Micromechanics Interdisciplinary Research Group (under the

Zeta potential

No—PEG

PEG

41.270.702 mV

12.870.208 mV

264

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

references

Assoian, Richard K., Klein, Eric A., 2008. Growth control by intracellular tension and extracellular stiffness. Trends Cell Biol. 18 (7), 347–352. Alfredo Uquillas, Jorge, Kishore, Vipuil, Akkus, Ozan, 2012. Genipin crosslinking elevates the strength of electrochemically aligned collagen to the level of tendons. J. Mech. Behav. Biomed. Mater.. Alenghat, Francis J., Fabry, Ben, Tsai, Kenneth Y., Goldmann, Wolfgang H., Ingber, Donald E., 2000. Analysis of cell mechanics in single vinculin-deficient cells using a magnetic tweezer. Biochem. Biophys. Res. Commun. 277 (1), 93–99. Bausch, Andreas R., Ziemann, Florian, Boulbitch, Alexei A., Jacobson, Ken, Sackmann, Erich, 1998. Local measurements of viscoelastic parameters of adherent cell surfaces by magnetic bead microrheometry. Biophys. J. 75 (4), 2038–2049. Christiansen, David L., Huang, Eric K., Silver, Frederick H., 2000. Assembly of type i collagen: fusion of fibril subunits and the influence of fibril diameter on mechanical properties. Matrix Biol. 19 (5), 409–420. Peter C.Y. Chen, Sahan C. Herath, Dong-an Wang, Kai Su, Kin Liao, Harry Asada. Active manipulation of uniaxial ecm stiffness by magnetic anchoring of bio-conjugated beads. In: ASME Summer Bioengineering Conference, pp. 1–14. Chippada, Uday, Yurke, Bernard, Georges, Penelope C., Langrana, Noshir A., 2009. A nonintrusive method of measuring the local mechanical properties of soft hydrogels using magnetic microneedles. J. Biomech. Eng. 131 (2), 021014 (021014). Chandrupatla, Tirupathi R., Belegundu, Ashok D., Ramesh, T., Ray, Chaitali, 1991. Introduction to Finite Elements in Engineering. Prentice-Hall, Englewood Cliffs, NJ. Peter C.Y. Chen, Sahan C.B. Herath, Dong-an Wang, Harry Asada. Active manipulation of ecm stiffness and its effect on endothelial cell migration during angiogenesis. In: Proceedings of the World Congress on Engineering, volume 1, 2012. Conrad-Lapostolle, V., Bordenave, L., Baquey, Ch, 1996. Optimization of use of uea-1 magnetic beads for endothelial cell isolation. Cell Biol. Toxicol. 12 (4–6), 189–197. Du, Yue, Herath, Sahan C.B., Wang, Qing-Guo, Asada, Harry, Chen, Peter C.Y., 2012. Analysis of stiffness in extracellular matrix embedded with bioconjugated magnetic beads in a magnetic field. Int. J. Biosci. Biochem. Bioinf. 2 (5), 329–335. Engler, Adam J., Sen, Shamik, Lee Sweeney, H., Discher, Dennis E., 2006. Matrix elasticity directs stem cell lineage specification. Cell 126 (4), 677–689. Elias, Paul Z., Spector, Myron, 2012. Viscoelastic characterization of rat cerebral cortex and type i collagen scaffolds for central nervous system tissue engineering. J. Mech. Behav. Biomed. Mater. 12, 63–73. Fratzl, Peter, Misof, Klaus, Zizak, Ivo, Rapp, Gert, Amenitsch, Heinz, Bernstorff, Sigrid, 1998. Fibrillar structure and mechanical properties of collagen. J. Struct. Biol. 122 (1), 119–122. Guillot, Pascale V., Cui, Wei, Fisk, Nicholas M., Julia Polak, Dame, 2007. Stem cell differentiation and expansion for clinical applications of tissue engineering. J. Cell. Mol. Med. 11 (5), 935–944. Guo, Cheng, Kaufman, Laura J., 2007. Flow and magnetic field induced collagen alignment. Biomaterials 28 (6), 1105–1114. Hansen, R.K., Bissell, M.J., 2000. Tissue architecture and breast cancer: the role of extracellular matrix and steroid hormones. Endocr. Relat. Cancer 7 (2), 95–113. Harland, Ben, Walcott, Sam, Sun, Sean X., 2011. Adhesion dynamics and durotaxis in migrating cells. Phys. Biol. 8 (1), 015011.

Helary, Christophe, Bataille, Isabelle, Abed, Aicha, Illoul, Corinne, Anglo, Annie, Louedec, Liliane, Letourneur, Didier, MeddahiPelle, Anne, Madeleine Giraud-Guille, Marie, 2010. Concentrated collagen hydrogels as dermal substitutes. Biomaterials 31 (3), 481–490. Sahan C.B. Herath, Peter C.Y. Chen, Yue Du, Shi Hui, Dong-an Wang, Qing-Guo Wang, Harry Asada. Active manipulation of ecm microscale stiffness. In: International Conference on Environmental, Biomedical and Biotechnology, volume 41, 2012. Hafeli, U.O., 2006. Magnetic nano and microparticles for targeted drug delivery. MML Series 8, 77. Keung, Albert J., Kumar, Sanjay, Schaffer, David V., 2010. Presentation counts: microenvironmental regulation of stem cells by biophysical and material cues. Annu. Rev. Cell Dev. Biol. 26, 533–556. Kane, Robert J., Roeder, Ryan K., 2012. Effects of hydroxyapatite reinforcement on the architecture and mechanical properties of freeze-dried collagen scaffolds. J. Mech. Behav. Biomed. Mater. 7, 41–49. Kaliske, Michael, Rothert, H., 1997. Formulation and implementation of three-dimensional viscoelasticity at small and finite strains. Comput. Mech. 19 (3), 228–239. Ludwig, Tenneille E., Bergendahl, Veit, Levenstein, Mark E., Yu, Junying, Probasco, Mitchell D., Thomson, James A., 2006. Feeder-independent culture of human embryonic stem cells. Nat. Methods 3 (8), 637–646. Lu, Jean, Hou, Runhua, Jane Booth, Carmen, Yang, Shih-Hung, Snyder, Michael, 2006. Defined culture conditions of human embryonic stem cells. Proc. Nat. Acad. Sci. U.S.A. 103 (15), 5688–5693. Lim, C.T., Zhou, E.H., Quek, S.T., 2006. Mechanical models for living cellsa review. J. Biomech. 39 (2), 195–216. Lipfert, Jan, Hao, Xiaomin, Dekker, Nynke H., 2009. Quantitative modeling and optimization of magnetic tweezers. Biophys. J. 96 (12), 5040–5049. Lodish, Harvey, 2008. Molecular Cell Biology. Macmillan. McNeish, John, 2004. Embryonic stem cells in drug discovery. Nat. Rev. Drug Discovery 3 (1), 70–80. Nakajima, Masafumi, Ishimuro, Toshinari, Kato, Koichi, Ko, InKap, Hirata, Isao, Arima, Yusuke, Iwata, Hiroo, 2007. Combinatorial protein display for the cell-based screening of biomaterials that direct neural stem cell differentiation. Biomaterials 28 (6), 1048–1060. Nilsson, Kurt, Mosbach, Klaus, 1981. Immobilization of enzymes and affinity ligands to various hydroxyl group carrying supports using highly reactive sulfonyl chlorides. Biochem. Biophys. Res. Commun. 102 (1), 449–457. Pelham, Robert J., Wang, Yu-li, 1997. Cell locomotion and focal adhesions are regulated by substrate flexibility. Proc. Nat. Acad. Sci. U.S.A. 94 (25), 13661–13665. Pedro Kato, Y., Christiansen, David L., Hahn, Rita A., Shieh, Goldstein, Jack D., Silver, Frederick H., 1989. Mechanical properties of collagen fiilve: a comparison of reconstituted and rat tail tendon fibres. Biomaterials 10 (1), 38–42. Raub, Christopher B., Suresh, Vinod, Krasieva, Tatiana, Lyubovitsky, Julia, Mih, Justin D., Putnam, Andrew J., Tromberg, Bruce J., George, Steven C., 2007. Noninvasive assessment of collagen gel microstructure and mechanics using multiphoton microscopy. Biophys. J. 92 (6), 2212–2222. Soen, Yoav, Mori, Akiko, Palmer, Theo D., Brown, Patrick O., 2006. Exploring the regulation of human neural precursor cell differentiation using arrays of signaling microenvironments. Mol. Syst. Biol. 2 (1). Stepanov, G.V., Abramchuk, S.S., Grishin, D.A., Nikitin, L.V., Yu Kramarenko, E., Khokhlov, A.R., 2007. Effect of a homogeneous magnetic field on the viscoelastic behavior of magnetic elastomers. Polymer 48 (2), 488–495.

journal of the mechanical behavior of biomedical materials 30 (2014) 253 –265

Savage, Brian, Komatitsch, Dimitri, Tromp, Jeroen, 2010. Effects of 3d attenuation on seismic wave amplitude and phase measurements. Bull. Seismol. Soc. Am. 100 (3), 1241–1251. Saffar, Saber, Abdullah, Amir, 2013. Longitudinal wave propagation in multi cylindrical viscoelastic matching layers of airborne ultrasonic transducer; new method to consider the matching layers diameter (frequency o100 khz). Ultrasonics. Stenkamp, Ronald E., Le Trong, Isolde, Klumb, Lisa, Stayton, Patrick S., Freitag, Stefanie, 1997. Structural studies of the streptavidin binding loop. Protein Sci. 6 (6), 1157–1166. Sofia, Susan J., Premnath, V., Merrill, Edward W., 1998. Poly (ethylene oxide) grafted to silicon surfaces: grafting density and protein adsorption. Macromolecules 31 (15), 5059–5070. Wells, Rebecca G., 2008. The role of matrix stiffness in regulating cell behavior. Hepatology 47 (4), 1394–1400. Wang, Yinling, Hu, Yuan, Chen, Lin, Gong, Xinglong, Jiang, Wanquan, Zhang, Peiqiang, Chen, Zuyao, 2006. Effects of

265

rubber/magnetic particle interactions on the performance of magnetorheological elastomers. Polym. Test. 25 (2), 262–267. Wang, Dong-an, Williams, Christopher G., Li, Qiang, Sharma, Blanka, Elisseeff, Jennifer H., 2003. Synthesis and characterization of a novel degradable phosphate-containing hydrogel. Biomaterials 24 (22), 3969–3980. Yanada, Shinobu, Ochi, Mitsuo, Adachi, Nobuo, Nobuto, Hiroo, Agung, Muhammad, Kawamata, Seiichi, 2006. Effects of cd44 antibody–or rgds peptide– immobilized magnetic beads on cell proliferation and chondrogenesis of mesenchymal stem cells. J. Biomed. Mater. Res. A 77 (4), 773–784. Zaman, Muhammad H., Trapani, Linda M., Sieminski, Alisha L., MacKellar, Drew, Gong, Haiyan, Kamm, Roger D., Wells, Alan, Lauffenburger, Douglas A., Matsudaira, Paul, 2006. Migration of tumor cells in 3d matrices is governed by matrix stiffness along with cell-matrix adhesion and proteolysis. Proc. Nat. Acad. Sci. U.S.A. 103 (29), 10889–10894.